covalent organic nanosheets for bioimaging mark a olson ... n2 adsorption/desorption ... mixture was
Post on 13-May-2020
Embed Size (px)
Covalent Organic Nanosheets for Bioimaging
Gobinda Das,[a]‡ Farah Benyettou,[a]‡ Sudhir Shrama,[b] Thirumurugan Prakasam,[a] Felipe Gándara,[c] Victor A. de la Peña -O’Shea,[d] Na'il Saleh,[e] Renu Pasricha,[a] Ramesh Jagannathan,[b] Mark A Olson[f] and Ali Trabolsi*[a]
a Chemistry Program, New York University Abu Dhabi (NYUAD), Experimental Research Building (C1), Saadiyat Island, United Arab Emirates b Engineering Division, New York University Abu Dhabi (NYUAD), Experimental Research Building (C1), Saadiyat Island, United Arab Emirates c Materials Science Factory, Instituto de Ciencia de Materiales de Madrid – CSIC, Sor Juana Inés de la Cruz 3, 28049 Madrid, Spain d Photoactivated Processes Unit, IMDEA Energy, Avd. Juan de la Sagra 3, Mostoles 28935, Madrid, Spain e Chemistry Department, College of Science, United Arab Emirates University, P.O. Box 15551, Al-Ain, United Arab Emirates f School of Pharmaceutical Science and Technology, Tianjin University, China
‡ Equal Contribution
Electronic Supplementary Material (ESI) for Chemical Science. This journal is © The Royal Society of Chemistry 2018
S1: General Material and Methods
S2: Synthetic procedure
S3. Fourier Transform Infrared (FTIR) Spectroscopy of the Synthesized TTA-DFP COF and TTA-DFP CONs Materials and their Precursors
S4: Thermogravimetric Analyses of TTA-DFP COF and TTA-DFP CONs
S5: Room Temperature PXRD Patterns of TTA-DFP CONs
S6: Pore Size Distribution of TTA-DFP COF.
S7: AFM Height Profiles of TTA-DFP COF and TTA-DFP CONs
S8: Room Temperature PXRD Patterns of TTA-DFP CONs
S9: Dynamic Light Scattering (DLS) Characterization
S10: AFM Height Profiles of TTA-DFP COF and TTA-DFP CONs
S11: HRTEM and AFM Analysis of TTA-DFP COF and TTA-DFP CONs
S12: Luminescent Study of TTA-DFP COF, TTA-DFP CONs and TTA-Monomer.
S13: Plane Wave Density Functional Theory (PW-DFT) Analysis
S14: Band Gap Calculations for UV-vis Spectra
S15: The Frontier Molecular orbital Distributions of TTA-DFP CONs Fragment by DFT Calculations
S16: Biological Studies
S1. General Materials and Methods
All reagents and starting materials were purchased from Sigma-Aldrich and used without further purification. The precursor, 2,6-diformylpyridine (DFP) was synthesized according to the published procedure with no modifications. Deionized water was used from Millipore Gradient Milli-Q water purification system. Thin-layer chromatography (TLC) was performed on silica gel 60 F254 (E. Merck). The plates were inspected under the UV light. Column chromatography was performed on silica gel 60F (Merck 9385, 0.040–0.063 mm). Routine nuclear magnetic resonance (NMR) spectra were recorded at 25 °C on a Bruker Avance spectrometer, with a working frequency of 500 and 125 MHz for 1H, and 151.0 MHz for 13C nuclei. All chemical shifts are reported in ppm relative to the signals corresponding to the residual non-deuterated solvents (CD3CN: = 1.94 ppm, CD3OD: = 3.31 ppm, D2O: δ = 4.97 ppm and DMSO-d6: δ = 2.50 ppm). Coupling constant values (J) are given in hertz (Hz), the multiplicity is abbreviated in the following way: s (singlet) and d (doublet). Fourier transform infrared (FTIR) studies were carried out on the Agilent 670-IR spectrometer. Thermogravimetric analysis (TGA) was performed on TA SDT Q600. Scanning electron microscopy (SEM) images were obtained from FEI Quanta 450FEG. The topography of the self-templated samples was analyzed by dynamic atomic force microscopy (5500 Atomic Force Microscope; Keysight Technologies Inc., Santa Rosa, CA). We acquired topography, phase and amplitude scans simultaneously. Silicon cantilevers (NanosensorsTM, Neuchatel, Switzerland) with resonant frequencies of 250–300 kHz and force constants of 100– 130 Nm−1 were used. The set point value was kept at 2.5V. AFM scans were collected at 1024 points/lines with scan speed of 0.20 at fixed scan angle of 0o. Scan artifacts were minimized by acquiring a typical scan at an angle of 90o under identical image acquisition parameters. We used GwyddionTM free soſtware (version 2.47), an SPM data visualization and analysis tool for post- processing the AFM scans. Size and morphology of the nanoparticles were determined with a TEM (FEI-Titan 300) microscope. Samples were prepared on a carbon-coated copper grid. A drop of dispersed polymeric network was spotted on the grid and allowed to dry overnight. UV-Vis studies were carried out on the Cary 5000 UV-Vis-NIR spectrophotometer. All UV-Vis spectra were recorded at room temperature in a quartz cell with 10 mm path length. N2 adsorption/desorption isothermal curves were both recorded at 273 K up to 1 bar using a manometric Micromeritics 3Flex gas sorption analyzer along with a PolyScience Circulating bath (50:50 vol%, water:ethylene glycol mixture) for maintaining constant temperature during the experiments. Powder X-ray diffraction (PXRD) measurements were carried out using the PANalytical X’Pert PRO MP X-ray diffractometer consisting of a focusing elliptical mirror and a fast high resolution detector (PIXCEL) with the radiation wavelength of 0.15418 nm.
The solid-state steady-state and time-resolved fluorescence measurements of polymers solid state and as a suspension (about 1 milligrams in 10 ml solvent) in different organic solvents (THF, 1,4- Dioxane, ethanol and water) were carried out using a solid sample holder, a LifeSpec II spectrometer that is based on the TCSPC method, excitation at 375 nm using an Edinburgh diode laser with a repetition rate of 20 MHz, a time resolution of 30 ps, and a red-sensitive high-speed PMT detector (Hamamatsu, H5773-04). Emission decays were collected every 10 nm over the entire emission spectra of TTA-DFP COF with a dwell time of 10 s at each wavelength. The data were globally fitted to a 3-exponential model function convoluted with instrument response function (IRF) of ~30 ps, utilizing Least-Square Statistical Analysis (x2) and residual plot are used to assess the goodness of fit).The time-resolved data were specifically analyzed using Edinburgh
FAST software in which decay-associated spectra (DAS) were constructed from the extracted intensity-contribution fraction (fi) calculated from the pre-exponential amplitudes (Bi), as follows:
𝐼(𝑡) = ∑ 𝑖
𝐵𝑖𝑒𝑥𝑝( ‒ 𝑡/𝜏𝑖)
𝑓𝑖 = 𝐵𝑖𝜏𝑖
Theoretical calculations by periodic density functional theory (DFT) were carried out using plane- wave calculations carried out using VASP1 package considering spin-polarization and dipole corrections explicitly. Geometry optimization was performed using the model obtained in the structure determination. The total energies corresponding to the optimized geometries of all samples were calculated using the spin polarized version of the Perdew−Burke−Ernzerhof (PBE) implementation of the GGA exchange correlation functional.2 The effect of the core electrons on the valence electron density was described by the project or augmented wave (PAW) method.3 In addition, the Heyd-Scuseria-Enzerhof hybrid functional (HSE06), with a mixing parameter of 0.225, was used to fit a more accurate energy gap. The cut-off for the kinetic energy of the plane- waves was set to 500 eV to ensure a total energy and force convergence better than 10−4 eV and 0.01 eV/Å3 respectively. The VESTA package v.39 was used to represent the charge density.4
Surface energy of the monolayer was calculated form DFT calculations of bulk and single layer nanosheet:
𝐸𝑆𝑢𝑟𝑓 = (𝐸𝑆𝑖𝑛𝑔𝑙𝑒 ‒ 𝐸𝐵𝑢𝑙𝑘)/3𝐴
Where ESurf is the surface energy and ESingle and EBulk are the energies form monolayer and bulk structures, A is de crystal surface and 3 is a factor to consider the number of layers including in the bulk structure.5
Theoretical optical properties were calculated using Time dependent Density Functional Theory (TD-DFT)6 implemented in the software Gaussian 09 7 employing a PBE0 functional.2 The standard 6–31G(d.p) basis set of double split valence plus polarization functions also on H atoms was chosen. Moreover, a fix number of 25 states were selected for a proper comparison between all configurations and models. Fluorescence images were obtained on an Olympus FV1000MPE confocal scanning microscope, images were taken with microscope power 60x.
S2: Synthetic Procedures
Synthesis of 2,6-diformylpyridine (DFP)
SeO2 (4.25 g, 38.0 mmol) was added with stirring to a solution of 2,6-pyridinedimethanol (5.5 g, 39.4 mmol) in dioxane (100 mL) in a 250-mL round-bottom flask fitted with a condenser. The mixture was then stirred under reflux condition for 20 h before adding charcoal (4 scoops) to the reaction mixture. The mixture was heated for an additional 10 min and filtered hot through celite bed. The filter cake was washed with dioxane (3 × 50 mL) and CH2Cl2 (3 × 50 mL). After combining the filtrates, the solvents were removed under reduced pressure and the residue was purified by column chromatography [SiO2: CH2Cl2] to afford DFP as a light pink solid. Yield: 77%; 1H NMR (500 MHz, CDCl3, 25 °C): δ 8.06 (t, 1H, J = 7.4 Hz, Ar-H), 8.17 (dd, 2H, J = 7.4 Hz, Ar-H), 10.16 (s, 2H, -CHO); 13C NMR (125 MHz, CDCl3, 25 °C): δ 125.3, 138.4, 153.0, 192.3.
4,4',4''-(1,3,5-triazine-2,4,6-triyl)trianiline (TTA): The triamine (TTA) was synthesized according to the published procedure with no modifications.8
Synthesis of TTA-DFP COF under Microwave condition: A microwave